Solid State Phenomena Vols. 95-96 (2004) pp. 415-420online at http://www.scientific.net© (2004) Trans Tech Publications, SwitzerlandJournal Citation (to be inserted by the publisher)Copyright by Trans Tech PublicationsFirst Principles simulations of extended defects atcubic SiC surfaces and interfacesA. Catellani 1 , G. Cicero 1,2 , G. Galli 3 , L. Pizzagalli 41 CNR-IMEM, Parco Area delle Scienze, 37a, I-43010 Parma, Italy, email@example.com INFM & Physics Department, Torino Polytechnic, Corso Duca Degli Abruzzi 24, I-10129 Torino,Italy, firstname.lastname@example.org Lawrence Livermore National Laboratori, POBox 808, Livermore, CA 94550, USA,email@example.com Laboratoire de Metallurgie Physique, CNRs & Univ. Poitiers, BP 30179, F-86962 FuturoscopeChasseneuil Cedex, France, firstname.lastname@example.orgKeywords: Silicon Carbide; Dislocations; Point Defects; Solid Surfaces and Solid-Solid Interfaces:Structure and Energetics; Molecular DynamicsAbstract. In this paper, we will review some recent investigations on extended defects in cubic SiC,as obtained from first-principles molecular dynamics. As an example of defects at surfaces, theformation of self-assembled nanowires, originating from coordination defects at the Carbonterminated SiC(001) surface is discussed. Furthermore, the mechanism governing the creation of anetwork of edge dislocations at the SiC/Si interface is presented. This system, characterized by apeculiar ~20% lattice mismatch, can be considered as a template of high lattice mismatchedheterostructures, where an ab initio approach is still affordable. We will discuss differences andsimilarities between the (001) and (111) interfaces, and compare our results with recentexperimental data.IntroductionSilicon carbide is a group IV compound semiconductor showing unique properties, that allow toconsider it as a true surface-science ‘laboratory’ : the charge polarization of the Si-C bondsmakes SiC a polar compound, midway between GaAs and ZnSe ; the existence of hundreds oftetrahedral SiC polytypes  rises fascinating fundamental problems and opens the way to manypotential technological applications. From the technological point of view, SiC is an extremelypromising semiconductor for high-pressure, high-temperature electronic devices, but also forbiological applications. The potentialities of SiC are severely affected by the large lattice mismatchwith most of the conventional substrates, that induces a poor control of growth, formation of pointand extended defects (dislocation and micropipes), but also low reproducibility of doping,metallization, surface preparation and stoichiometry. Several studies have recently been devoted tothe understanding, characterization and technological exploitation of SiC properties, and a numberof publications and review papers appeared on the theoretical study of point defects [4,5], surfaceproperties [2,3,6], and interface structure [7,8] in SiC. Here, without presumption of completeness,we will present the latest results of first-principles simulations on the formation mechanism,energetics and local structure of extended defects at cubic SiC surfaces and interfaces. We willfocus on selected systems, where the availability of recent experimental data complete the scenarioand allows to show the complementarity between the experimental and theoretical approaches.All rights reserved. No part of contents of this paper may be reproduced or transmitted in any form or by any means without thewritten permission of the publisher: Trans Tech Publications Ltd, Switzerland, www.ttp.net. (ID: 126.96.36.199-17/09/07,10:17:11)
416Gettering and Defect Engineering in Semiconductor Technology X2 Title of Publication (to be inserted by the publisher)MethodThe present paper deals with first principles molecular dynamics simulations of electronic andstructural properties of defects in SiC: the method  allows for a combined relaxation of both theionic and electronic degrees of freedom towards the ground state configuration. Calculations areperformed in the supercell approach within the Density Functional Theory (DFT), in the LocalDensity Approximation (LDA); the problem of coordination defects and self-assembled C-wireshowever requires the use of GGA . An energy cutoff of at least 40 Ry is used for the planewaves expansion of the wavefunctions, depending on the pseudopotential choice . Thereciprocal space integration in the Brillouin Zone (BZ) is done by considering only the point ofthe supercell. The lateral dimensions of the supercell are chosen big enough to provide a goodsampling of the BZ, and non interacting defect replicas ; furthermore, a wide (> 8 ) vacuumspace is included to avoid spurious surface-surface interaction between supercell replicas.Calculations are always performed at the theoretical equilibrium lattice parameter, consistent with¡the chosen pseudopotentials. Structures are considered converged when forces acting on atoms areless than 10 -4 a.u. (0.005 eV/Å) and energy varies by less than 10 -5 eV/atom. Further details on themethod used can be found in [5,6,12] for the SiC(001) surfaces, and in  for the SiC/Si interface.Self-assembled nanowires (sp 3 coordination defects) at C-SiC(001)Recent experiments  have shown that stable sp 3 -like bonded carbon lines can be formed on theC-terminated SiC(001) surface [14,15], by inducing an irreversible sp¢ sp 3 phase transition in thesubstrate. These sp 3 lines point at possible precursors for diamond growth on SiC surfaces, andpossibly at enhancing the SiC biocompatibility.Motivated by these recent experiments , we simulated the appearance of coordination defectson the C-SiC(001)-c(2x2) reconstructed surface. Starting from the ideal geometry of thisreconstruction, we arbitrarily rotated some C-dimers by 90° thus inducing a local sp¢ sp 3 transition.The calculations were performed at different defect densities, £ = 1/8, 1/4, 1/2. The defectformation energy, which is 1.2 eV/dimer at £ = 1/8, decreases rapidly when more defects arecreated at the surface, and is ~ 0.05 eV/dimer at £ = 1/2, in good agreement with the experimentalfindings, showing that sp 3 dimers are more probable at high defect concentrations. Our ab initioresults provide further details on the structural and electronic properties of the defects, that cannotbe achieved in experiment: the sp 3 defects (see Fig.1), which always lie below the sp pattern ofapproximately 0.4 Å, are unbuckled, with dimer bond length of 1.36-1.38 ¡ , depending on defectconcentration. Although the sp-dimers bond length is unaffected by the presence of the sp 3 dimer,the overall sp chain geometry is modified, accordingly to the strain associated with the presence ofthese rotated coordination defects.The sp 3 defect conformation which results from our calculation is in apparent disagreement withthe experimental observation  of asymmetric sp 3 dimers lying above the sp chains, as inferredfrom the measured STM images. In order to make contact with experiment, we have calculated bothfilled and empty states STM images of the defected surface. We have found two surface stateslocalized on the defects, and separated by a gap of 0.2 eV. These states have the same symmetry andorbital character as the HOMO and LUMO surface states found in the p(2x1) reconstruction .The STM images (Fig. 1-a) computed using the Tersoff-Hamman approximation  are in verygood agreement with the experimental ones (Fig. 1-b): the apparent buckling induced by chargedistribution in the neighborhood of sp 3 -like bonded carbon atoms strictly resembles its experimentalcounterpart.We have furthermore evaluated the effect of the presence of other defects on the formationenergy of the sp¢ sp 3 coordination defect: to this aim, we studied a symmetric slab with a missing
Solid State Phenomena Vols. 95-96 417sp dimer at both surfaces close to the coordination defect and optimized the atomic and electronicstructures of the supercell. In this case the formation energy of the sp 3 defect is approximately seventimes lower than on a clean surface with no missing dimers. These results indicate that occasionalmissing units on the C-SiC(001)-c(2x2) surface may represent local seeds for the sp to sp 3 transitionobserved experimentally.The SiC/Si interfaceAnother example of application of first-principles calculations to complement and interpret theexperimental results is provided by the large scale simulations of the SiC/Si(001) interface .Thanks to the large lattice mismatch of ~ 20%, this interface may be considered as a model of highlattice mismatch heterostructure of covalent materials, where ab initio simulations are stillaffordable.Notwithstanding the high mismatch, SiC can be grown on Si(001), using different techniques[7,17,18]; the microscopic description of the interface is however incomplete. Classical  and abinitio  molecular dynamics simulations indicate that pseudomorphic thin SiC films cannot begrown on Si: our investigations  on the stability of few (1-3) SiC bilayers on Si(001) show thatSiC never grows in pseudomorphic, defect free films on this substrate, and eventually amorphousSiC layers are found to be more stable. An efficient mechanism of strain relief must be at work atthe very first stages of growth to obtain an abrupt interface, and epitaxial SiC films.A recent High-Resolution Electron Microscopy (HREM) study of this system evidenced a locallyabrupt interface, with the presence of a periodic array of misfit dislocations . These ones seemto be pinned at the interface, which points at a vanishing critical thickness for this heterostructure.Still it is diffcult to gain additional information from these experiments. In particular, the atomicstructure and the chemical environment at the interface, which deeply affect its physical properties,remain hardly accessible.In order to provide a thorough description of the system, we have performed a combined classicaland first-principles molecular dynamics study to investigate the stoichiometry of the interface aswell as its stability . We first performed a structural optimization for several possible interfaceconfigurations, varying both geometry and stoichiometry, via classical molecular dynamics, in orderto get the most stable structure. Slab sizes up to 60 SiC and 60 Si layers were considered. The Si-Si,Si-C, and C-C interactions were modeled by means of the empirical Tersoff potentials . Therelative energy of systems containing different numbers of atoms were compared in the grandcanonical scheme . Our classical results indicate that configurations with C atoms at theinterface are always more stable. In agreement with experimental results , the favored corestructures are those with the dislocations pinned at the interface, which corresponds to a vanishingcritical thickness.The classical MD analysis allowed us to select the core dislocation structures and slab size forthe ab initio simulations. Since the relative atomic distortions are less than 2% after the 4th layer,when considering a 7/7 or a 60/60 layer slab, and the 7/7 slab reproduces correctly the asymptoticvalue of an infinite (60/60) system, the ab initio simulations were performed on a 7/7 layer slab.Among all the considered geometries, our first-principles simulations were performed only for themost meaningful ones: the stoichiometric interface and the one which is lowest in energy. The latter(see Fig.2, left) is obtained from the stoichiometric solution by removal of all the C atoms along thetwo core dislocation lines (13 atoms per supercell): this configuration is 5.69 (15.05) eV/cell lowerin energy than the stoichiometric one in C-rich (C-poor) conditions respectively, in the case of a 7/7layers slab.The analysis of the configuration topology gives some hints for understanding this result. The setof classical calculations has indeed shown that it is preferable to have C atoms at the interface in thefirst SiC layer, although the stretching of carbon bonds is energetically expensive. In this
418Gettering and Defect Engineering in Semiconductor Technology X4 Title of Publication (to be inserted by the publisher)reconstructed interface, with an understoichiometric carbon layer, the first SiC layer is carbon-like,but there is only one C atom involved in the reconstructed dislocation cores. It also presents thepeculiar characteristics that almost no atoms are sub- or over-coordinated, owing to the formation ofa topological ring along one direction and the formation of a silicon dimer along the other. Thisconfiguration is then the best candidate to represent the atomic structure of the SiC/Si(001)interface. A qualitative indication of the residual strain distribution at the interface can be obtainedby inspection of the deformation of the converged system coordinates, with respect to the idealbulk-like positions. Fig. 2 represents the residual strain field at the interface for this geometry,evaluated in terms of atomic displacements from ideal bulk-like positions. As it is evident fromsimple inspection, the major deformations are localized in Si, which has smaller elastic constantsthan SiC. This result, along with the occurrence of a periodic dislocation network, has been recentlyconfirmed by accurate High Resolution TEM experimental  and simulated  images. Adetailed description of the structure and energetics of the several configurations studied is reportedelsewhere .The ab initio simulations, although providing a deeper insight and structural and electronicdetails that remain prohibitive in empirical calculations, validate the results obtained by classicalmoleculardynamics. Based on these findings, we studied also the SiC/Si(111) interface: because of the largesupercell size requested by the hexagonal lattice, we performed in this case only classicalsimulations . The (111) surface of a zincblende crystal can be obtained either with a shuffle or aglide plane which differ for stability and number of dangling bonds; at a (111) interface the situationis furthermore complicated by the possibility of having an inversion in the layer stacking sequence.A number of different configurations have been considered thus sampling the configuration spacefor this interface. We first investigated the possibility of forming stoichiometric interfaces bymatching a Si and a SiC layers with different terminations at the interface: two shuffle planes, twoglide planes or a shuffle and a glide plane were considered. Our results indicate that interfacesbetween shuffle planes are always more stable. Furthermore, similarly to what was found for theSiC/Si(001) system, our calculations revealed that it is always favorable to have carbon at theinterfaces. We also considered the possibility of having pseudomorphic SiC grown layers, beforethe dislocations start, which was found to be an unfavorable configuration. Thus, as in the β-SiC/Si(001) interface, the dislocation cores are directly pinned at the interface, in agreement withexperimental evidence .The dislocation core for the most stable stoichiometric interface structure is presented in Fig. 3.The structure presents under-coordinated C atoms forming three SiC bonds 1.80 Å long in adistorted sp 2 hybridisation. At variance with the SiC/Si(001) system, structures obtained eliminatingthe unsaturated and distorted atoms are higher in energy. We finally analysed the possibility ofhaving a stacking inversion at the interface, which would lead to a SiC crystal structure mirroredwith respect to the previous one. We found that the energy difference between the two structureslays in the error bar of our calculation, resulting than degenerate. Twins are thus likely to formdirectly at the Si(111) surface, as indeed revealed by recent HREM dark field micrographs [18,25].SummaryIn conclusions, the two examples of ab initio simulations of extended defects in SiC presented inthis work evidence the capability of the method in complementing the experimental result, andprovide a microscopic description of the defect structure. In particular, for the SiC/Si interface,which can be considered as a template of high lattice mismatched heterojunctions, the large scalecalculations required to describe the dislocation network, are in very nice agreement with newestexperimental results.
Solid State Phenomena Vols. 95-96 419AcknowledgmentsWe are indebted to a number of coworkers, and we are especially grateful to Stefano Frabboni andVincenzo Grillo for providing us their TEM experimental data and simulations prior to publication,and for helpful discussions.The work was partially supported by INFM through the projects PRA:1MESS and ParallelComputing Initiative; calculations were performed in CSCS (Manno-CH), IDRIS (Orsay, F),CINECA (Bologna-I) and CICAIA (Modena-I).References V. Bermudez, Nature Materials, 2 (2003), in print. M. Sabisch, P. Krueger, and J. Pollmann, Phys. Rev. B 51(1995), p.13367; J. Pollmann, P.Krueger, and M. Sabisch, Phys. Stat. Sol. (b) 202 (1997), p. 421; J. Pollmann, et al., Appl.Surf. Sci. 104-105(1996), p.1. F. Bechstedt, et al., Phys. Stat. Sol. (b) 202 (1997), p. 35; F. Bechstedt and P. Kaeckell, Phys.Rev. Lett. 75 (1995), p. 2180; P. Kaeckell, J. Furthmueller, and F. Bechstedt, Phys. Rev. B 60(1999), p.13261. F. Gao, et al., Phys. Rev. B 64 (2001), p. 5208; L. Torpo, et al., Appl. Phys. Lett. 74 (1999),p.221; F. Bechstedt, A. Zywietz, J. Furthmuller, Europhys. Lett. 44 (1998), p.309; T.Wimbauer, et al., Phys. Rev. B 56 (1997), p.7384; L. Torpo, S. Poykko, R.M. Nieminen, Phys.Rev. B 57 (1998), p.6243; C. Wang, J. Bernholc, R.F. Davis, Phys. Rev. B 38 (1988), p.12752. A. Catellani, and G. Galli, Diamond & Rel. Mat. 10 (2001), p.1259. A. Catellani, and G. Galli, Prog. Surf. Sci. 69 (2002), p.101. M. Kitabatake, Thin Solid Films 369, (2000), p.257; V. Chirita, L. Hultman, and L. R.Wallenberg, Thin Solid Films 294 (1997), p.47. G. Cicero, L. Pizzagalli, and A. Catellani, Phys. Rev. Lett. 89 (2002), p.156101. We used the first principles molecular dynamics programs BASIC96 and JEEP (G. Galli and F.Gygi). For a review see, e.g., G. Galli and A. Pasquarello, in Computer Simulation in ChemicalPhysics, Edited by M.P.Allen and D.J.Tildesley, p. 261, Kluwer, Dordrecht (1993); and M. C.Payne, et al., Rev. Mod. Phys. 64 (1993), p.1045. J.P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett. 77 (1996), p. 3865. D. Hamann, Phys. Rev. B 40 (1989), p.2980. Calculations performed with GGA exchange andcorrelation  required a larger cutoff of 80 Ry. In the case of the dislocation network, thelong tailed stress field induces of course an interaction between the replicas. The supercelllateral dimensions are in this peculiar case dictated by the near-coincidence lattice model: aperfect coincidence site between two dissimilar structures of lattice parameters a1 and a2,respectively, is realized when a1/a2 =m/n, with m and n positive integers. For the cubic SiC/Sisystem, m=5 and n=4: this gives 25 (16) atoms/layer in the SiC (Si) part of the slab. A. Catellani, G. Galli, and P.L. Rigolli, Phys. Rev. B. 62, (2000) p.R4794. V. Derycke, et al., Phys. Rev. Lett. 81 (1998), p.5868. A. Catellani, G. Galli, F. Gygi, Phys. Rev. Lett. 77 (1996), p.5090. V.M. Bermudez, Phys. Stat. Sol. b 202 (1997), p.447 ; J. Long, V. Bermudez, and D. Ramaker,Phys. Rev. Lett. 76 (1996), p.991. J. Tersoff, D. Hamann, Phys. Rev. B 31 (1985), p.805. S. R. Nutt, D. J. Smith, H. J. Kim, and R. F. Davis, Appl. Phys. Lett. 50 (1987), p.203; Q.Wahab, et al., Appl. Phys. Lett. 65 (1994), p.725; M. Kitabatake, Thin Solid Films 369 (2000),p.257. C. Long, S. A. Ustin, and W. Ho, J. Appl. Phys. 86 (1999), p.2509.
420Gettering and Defect Engineering in Semiconductor Technology X6 Title of Publication (to be inserted by the publisher) G. Cicero, Ph.D. Thesis: “Ab initio simulations of -SiC growth on Si(001): from atomicadsorption to the buried interface”, Torino Polytechnic, April (2003). J. Tersoff, Phys. Rev. B 39 (1989), p.5566. G. X. Qian, R.M. Martin, and D. J. Chadi, Phys. Rev. B 38 (1988), p.7649. S. Frabboni, private communication. V. Grillo, et al., Institute of Physics Conference Series in press(2003). L. Pizzagalli, G. Cicero, and A. Catellani, Phys. Rev. B, submitted (2003). K.Tanaka and M. Kohyama, Phil. Mag. A 82 (2002), p.215.